electroannealing: Supplemental Material
Simon Collienne,1, ∗ Bart Raes,2 Wout Keijers,2 Julian Linek,3 Dieter Koelle,3 Reinhold
Kleiner,3 Roman B. G. Kramer,4 Joris Van de Vondel,2 and Alejandro V. Silhanek1, †
1Experimental Physics of Nanostructured Materials, Q-MAT,
CESAM, Universit´e de Li`ege, B-4000 Sart Tilman, Belgium
2Quantum Solid-State Physics, Department of Physics and Astronomy,
KU Leuven, Celestijnenlaan 200D, B-3001 Leuven, Belgium
Physikalisches Institut, Center for Quantum Science (CQ) and LISA+, Universit¨at T¨ubingen, D-72076 T¨ubingen, Germany
4Universit´e Grenoble Alpes, CNRS, Grenoble INP, Institut N´eel, 38000 Grenoble, France
(Dated: January 27, 2021)
I. IN SITU SCANNING ELECTRON
Fig. SM-1(a) shows the maximum resistance (Rmax)
obtained at a current IEA and the minimum resistance
(Rmin) obtained after the current has been switched off
for a supplementary sample. For IEA ≤ 10 mA, the
in-crease of Rmaxwith increasing IEAresults primarily from
Joule heating, as confirmed by the fact that no change of Rminis observed in this current range. IEA = 10 mA
rep-resents the threshold beyond which irreversible modifica-tions in the constricmodifica-tions are induced. For each EA step depicted in Fig. SM-1(a), we have acquired SEM images after the device has been submitted to thermal stress. A selected set of these images are shown in Fig. SM-1(b) to (e). Fig. SM-1(f) and (g) show a zoom in of the two con-strictions on Fig. SM-1(e) where clear surface damage, preferentially occurring on the I- side, can be observed. One can note that no apparent structural modification are revealed for IEA ≈ 10 mA whereas clear material
alteration localized at both constrictions are seen after exceeding the threshold current. The affected area is about 4200 nm2 and 6300 nm2for upper and lower
II. FINITE ELEMENT METHOD SIMULATION
Considering the non-trivial geometry of the system, the temperature inside the SQUID at low bath tem-perature for increasing current during the Joule heating regime has been estimated by the finite element method (FEM) based simulation software COMSOL . The model assumes the 50 nm-thick Nb sample in contact with a 100 nm silicon oxide layer on top of a pure 100 x 100 x 30 µm3 silicon wafer. The software resolves the heat transfer equation :
ρmC ∂T ∂t = κ∇ 2T + Q (1) ∗firstname.lastname@example.org †email@example.com
with ρm the density in kg/m3, C the specific heat
ca-pacity in J/(kgK), T the temperature in K and κ the thermal conductivity in W/(Km). The last term in (1) is determined by the Joule heating
Q = j · E = ρj2 (2)
with ρ the electrical resistivity in Ωm. For the stationary solution, the left hand side term of (1) vanishes. The parameters used in the simulations are summarized in Table SM-1. The thermal conductivity for Nb is taken from the bulk properties of the material. Although this value probably overestimates the real thin film value of κ , the increase in temperature was rather insensitive to this parameter.
κ [W/(mK)] ρ [µΩcm] α [K−1]
Nb 54 9.57 8.5 × 10−3
SiO2 1.4 1023 /
Si 130 1.22 × 106 /
Table SM-1. Thermal conductivity, electrical resistivity and thermal coefficient as input parameters in COMSOL simula-tions.
The model includes a thermal contact at two interfaces between all three layers by forcing heat fluxes to obey:
q⊥,12= −h(T )(T2− T1) (3)
where q⊥,12 is the heat flux in W/m2 from medium 1
to medium 2 and h(T ) the temperature-dependent heat transfer coefficient in W/(Km2).
The main panel of Fig. SM-2 plots the evolution of the resistance as a function of current at a bath temperature Tb = 10 K. At low bias current, thermal dissipation is
low and the temperature throughout the SQUID is ho-mogeneous and equal to Tb. At larger currents the heat
generation cannot be evacuated fast enough hence lead-ing to an inhomogeneous temperature distribution and higher resistance. Since the temperature increases by several hundred of Kelvins during the electroannealing process, a temperature dependence of the heat transfer coefficient h(T ) = a+bT3where a = 2.99×106W/(m2K)
Figure SM-1. SEM images obtained during the electroannealing process for sample S2. Panel (a) shows the values of the maximum resistance (Rmax) in red color obtained at a current IEAand the minimum resistance (Rmin) in blue color obtained
after the current has been switched off. Starting from pristine state (b) EA runs produce no apparent structural modification until reaching EA10 (e). Panels (f) and (g) show a zoom-in of both Dayem bridges in panel (e). Scales bars in (b) and (g) correspond to 200 nm and 100 nm, respectively.
and b = 12.6 W/(m2K4) are determined in order to
repro-duce the experimental results. The spatial distribution of temperature, given in the inset of Fig. SM-2 for I = 9 mA at the end of the reversible Joule heating regime, shows a substantial rise of temperature in the entire SQUID (∼ 400 K) and not only in the bridges (∼ 460 K).
III. IN SITU ATOMIC FORCE MICROSCOPY
As can be seen in Fig. 3 of the main text, the width of the lower bridge decreases from the pristine state to panel (c). This clear tendency to shrink leads us to believe that this phenomenon may be accompanied by overgrowth perpendicularly to the plane of the SQUID. In order to re-veal these features, otherwise concealed by top-view SEM images, we used in situ atomic force microscopy (AFM) permitting a vertical resolution of 0.1 nm. Fig. SM-3 shows a set of AFM images acquired in tapping mode at ambient conditions and for three consecutive stages of EA. As electroannealing progresses and the resistance of the device increases, a clear overgrowth develops simulta-neously in both junctions achieving a height excess of 17 nm. The observed overgrowth at the constrictions could also result from the formation of Nb2O5 since the AFM
images were acquired at atmospheric condition unlike the SEM images presented in Fig. 3 of the manuscript.
8400 I = 9 mA 300 200 100 [K] I = 9 mA 400 300 200 100 (K)
Figure SM-2. Resistance rise as a function of increasing cur-rent (sample S1) for the curcur-rent range where the R(I) is solely affected by Joule heating. The blue curve represents the ex-perimental data and red squares are results from FEM simu-lations. The inset shows the temperature profile in the bridge for I = 9 mA just before EA starts.
The AFM observations were carried out in a Multimode-8 atomic force microscope at room tempera-ture and in air with standard silicon tapping mode probe
Rmin = 22 Ω Rmin = 86 Ω Rmin = 151 Ω
Figure SM-3. AFM images taken after three consecutive stages of electroannealing at room temperature (sample S5). The scale bar corresponds to 200 nm.
with reflex aluminium coating on the detector side of the cantilever. A 10 nm radius of curvature tip with a can-tilever of 42 N/m nominal spring constant was used with a lateral scan rate of 1 Hz at 512 lines.
IV. WEAK LINKS SUPERCONDUCTING
10Virgin EA05 EA07 EA08 EA10 EA12 EA14
Figure SM-4. (a) R(T ) evolution for sample S4. (b) Resis-tance of the normal state and critical temperature taken for (a) and plotted as a function of EA number.
Fig. SM-4(a) shows a selected set of R(T ) curves taken after various EA steps on sample S4. The measured nor-mal resistance and critical temperatures are summarized in Fig. SM-4(b) and present clear similarities with re-spect to the results shown in the main text for sample S1 (Fig. 4), demonstrating good reproducibility of the EA effects on sample behaviour.
V. COHERENCE LENGTH EVOLUTION OVER
Since the EA process leads to a modification of the material properties as well as the geometry of the con-strictions, it is important to know if the superconduct-ing coherence length ξ at the weak links is also af-fected. In order to tackle this question, we measured the superconducting-normal phase boundary Bc2(T )
af-ter each EA step. Fig. SM-5(a) shows the R(B) curves measured at T = 1.8 K after four EA steps. Subsequent EA steps result in a reduced Bc2 value of the weak link
characterized by a kink in the R(B) curves of EA08 and EA14 as indicated by the black arrows. This kink disap-pears for EA11, which corresponds to an EA step at al-most maximum recovery, resulting in a R(B) very close to the pristine state. A set of phase boundaries is shown in Fig. SM-5(b) together with the linear fits corresponding to Bc2(T ) = Φ0/(2πξ(T )2) with ξ(T ) = ξ(0)/p1 − T /Tc
and Φ0≈ 2.0678 mTµm2 is the magnetic flux quantum.
Similarly as for the R(T ) curves, we used a criterion of 0.9RN to determine Bc2 of the SQUID arms and 0.1 Ω
for estimating Bc2at the weak links. Note that the phase
boundary first shrinks as superconductivity at the weak link is deteriorated and then recovers towards to the ini-tial pristine state, in agreement with the data presented in Fig. SM-4. Fig. SM-5(c) summarizes the results of the fitting and shows that the superconducting coherence length at the weak links ξ0(0) remains nearly unaffected by the EA process up to EA10, whereas for further EA processes, ξ0(0) tends to grow.
-2 0 0 2 -2 -4 4 2 2 4 6 8
Bc2 (T)0 8 10 12 14
)(c) EA00 EA08 EA11 EA14 (a) (b) 5 10 4 6 8
EA numberξ(0) ξ'(0) T'C TC 0 5 10
Figure SM-5. (a) Resistance vs applied magnetic field B at T = 1.8 K and for four different stages of EA (sample S4). EA00 corresponds to the pristine state. (b) Phase boundaries Bc2(T ) for the SQUID arms (black crosses), the constriction
in the pristine state (black circles), after EA08 (red squares), EA11 (orange stars) and EA14 (green stars). In panel (c) the critical temperature Tc0and the coherence length ξ
(0) of the weak links are compared with those corresponding to the SQUID arms (Tc and ξ(0)) after each EA step.
VI. DYNAMIC THERMAL MODEL
Recently, a time dependent thermal model for a weak link made of a superconducting constriction was pro-posed by Gupta et al. . The model describes several thermal regimes mainly determined by the heat evac-uation efficiency. These authors identified a dynamic regime where a non-zero voltage exists across the weak link when its temperature stabilizes between the bath temperature and the superconductor’s critical tempera-ture. The model was successfully applied to Nb based nanoSQUIDs biased at different currents . In this section we implement EA processing as a way to pro-gressively affect the thermal properties of the weak link. The thermal response of the system is ruled by a single parameter,
which quantifies the ratio between the Joule heating and the heat evacuation. In Eq.(4), RN is the normal
re-sistance of the two weak links in parallel, Ic(Tb) is the
critical current of the whole device at the bath temper-ature Tb and k the heat loss coefficient in W/K from
the weak link through the bulk electrodes and interfaces.
Similar dimensionless parameters have been introduced in Ref.[42, 43]. For the case of a short weak link (d ξ), and assuming a linear temperature dependence of the critical current and a temperature independent k, the β parameter is linked to the retrapping current Ir and
critical current Ic as follows :
I r Ic 2 = p 1 + 4β4− 1 2β2 . (5)
This equation allows us to determine β as a function of temperature as shown in Fig. SM-6(a). From the ob-tained β(Tb) and the experimentally determined RN, Ic
and Tc, we can deduce k.
The practical application of this model requires an es-timation of the value of RN. According to Ref. the
retrapping current Ir(T ) = 2p2g(T )L0Tc/RN, with L0
the Lorenz number, RN the normal resistance of the two
Josephson junctions in parallel and g(T ) a non-linear function of temperature related to the thermal conductiv-ity in the superconducting state. Using only RN as free
fitting parameter we obtain RN ≈ 6.2 Ω. Since EA
mod-ifies RN, a new estimation needs to be done after each
EA step. In order to do so, we assume, as confirmed by SEM and AFM measurements, that all EA modifications are located at the constrictions and that the affected area does not substantially change in size. The total normal resistance is simply given by R = Rarms + RN where
Rarms is the resistance of the two arms of the SQUID in
parallel. Under these assumptions, we are able to esti-mate the resistance of the arms from the pristine state: Rarms= Rpristine− RN = 1.72 Ω, which is assumed to
re-main invariant for subsequent EA processes. After each EA step, we measure R and deduce RN as shown in the
inset of Fig. SM-6(c).
To obtain an estimation of the heat loss coefficient k, we fit the experimental values of β(Tb) with Eq.(4) using
k as single fitting parameter. Fitted curves assuming a temperature-independent k are shown for EA00, EA07 and EA08 in Fig. SM-6(a), (b) and (c), respectively. For EA steps characterized by a high critical current (EA00 → EA06), the model is unable to reproduce the β(Tb)
curve with a temperature-independent k (Fig. SM-6(a)). The observed discrepancy between the theoretical model and the experimental data at low temperatures is likely due to the high value of the critical current which gives rise to substantial Joule heating for which the assumption of k being temperature-independent is no longer valid. For EA07, the dynamic thermal model is able to capture already the main features of the β(Tb) dependence using
a temperature-independent k parameter (Fig. SM-6(b)). From EA08 until EA10 the fitted curve perfectly overlaps the experimental values as can be seen for EA08 in the main panel of Fig. SM-6(c) and the obtained kopt= 11.9
nW/K is of the same order of magnitude than the values reported by Biswas et al.  for Nb SQUIDs. After EA10, the sample becomes totally nonhysteretic and, ac-cording to Eq.(5), β = 0 for all temperatures, meaning
EA00 EA07 EA08 2 4 6 80 200 400 600 k (n W/K) Tb (K) Tb (K) (a) (b) (c) EA00 (d) EA01 EA02 EA03 EA06 EA07 EA08 EA09 EA10 Exp. Best �it 14 12 10 8 6 40 5 10 15 EA number Rn ( Ω ) kopt = 11.9 nW/K 0 50 100 6 5 4 3 2 8 6 4 2 80 60 40 20 0 40 30 20 10 0 2 2.5 3 3.5
Figure SM-6. Dynamic thermal model results for sample S4. (a), (b) and (c) give experimental values of β for EA00, EA07 and EA08 respectively and the corresponding optimum kopt.
Inset of (c) indicates the evolution of the resistance of the two weak links in parallel under the assumption cited in the text. (d) Evolution of k(Tb) for all EA steps. Note the green
curve of EA07 that divide the EA steps in two distinguished thermal regimes.
that heat evacuation is always sufficient to avoid ther-mal runaway in the SQUID. As we will show below, the trend towards a nonhysteretic behavior is not caused by an improvement of k but rather is a consequence of the rapid decrease of Ic. Assuming that the failure of the
dynamic thermal model for the initial EA steps arises from the breakdown of the temperature independence of k, we can instead calculate for each temperature and each EA steps, the value of k(Tb) directly given by eq.(4) (see
Fig. SM-6(d)). The observed k(Tb) dependence indicates
that the heat evacuation in the SQUIDs switches from a good heat evacuation regime before EA07 to a less ef-fective one after EA07. Within these two regimes, k(Tb)
seems to be rather independent of the EA number. Yet, as can be seen in Sec. IV, EA07 is precisely the run where the normal resistance increases and the critical tempera-ture decreases, indicating that the significant k reduction is owing to a structural modification in the sample.
 S. Biswas, C. B. Winkelmann, H. Courtois, and A. K. Gupta, ”Josephson coupling in the dissipative state of a thermally hysteretic µ-SQUID,” Phys. Rev. B 98 (2018).  A. K. Gupta, N.l Kumar, and S. Biswas, ”Tempera-ture and phase dynamics in superconducting weak-link,” J. Appl. Phys. 116, 173901 (2014).
 COMSOL Multiphysics v. 5.4. COMSOL AB, Stock-R
 A. D. Avery, S. J. Mason, D. Bassett, D. Wesenberg, and B. L. Zink, ”Thermal and electrical conductivity of approximately 100-nm permalloy, Ni, Co, Al, and Cu films and examination of the Wiedemann-Franz Law,”
Phys.Rev. B 92 (2015).
 A. V. Gurevich and R. G. Mints, ”Self-heating in normal metals and superconductors,” Rev. Mod. Phys. 59, 941-999 (1987).
 X. D. A. Baumans, V. S. Zharinov, E. Raymenants, S. Blanco Alvarez, J. E. Scheerder, J. Brisbois, D. Massarotti, R. Caruso, F. Tafuri, E. Janssens, V. V. Moshchalkov, J. Van de Vondel, and A. V. Silhanek, ”Statistics of localized phase slips in tunable width pla-nar point contacts,” Sci. Rep. 7, 44569 (2017).
 D. Hazra, J.R. Kirthley, and K. Hasselbach, ”Retrapping Current in Bridge-Type Nano-SQUIDs,” Phys. Rev. Appl. 4, 024021 (2015).